Cement-Based Pavement Materials Water Content Cement Content Cast Rolled No Wearing Course Required Wearing Course Required Roller-Compacted Concrete Conventional Concrete Soil-Cement Flowable Fill Cement-Modified Soil Full-Depth Reclamation Cement- Treated Base Pervious Concrete
Hydration Products all particles not coated voids not filled linkages bind soil agglomerations together Cementitious Gel or Paste coats all particles fills voids Concrete Soil-Cement
Definition of Full-Depth Reclamation Method of flexible pavement reconstruction that utilizes the existing asphalt, base, and subgrade material to produce a new stabilized base course for a chip seal, asphalt, or concrete wearing surface.
Surfaced Roadways in the United States (2,495,000 total centerline miles) Composite Rigid Flexible
Challenges Facing Our Roadways Continuing growth Rising expectations from users A heavily used, aging system Environmental compatibility Changes in the workforce Funding limitations Combined with large increases in traffic volumes and/or allowable loads often leads to serious roadway base failures!
How do you know if you have a base problem and not just a surface deficiency?
Examples of Pavement Distress Alligator cracking Rutting Excessive patching Base failures Potholes Soil stains on surface
Use of in-place materials Little or no material hauled off and dumped Maintains or improves existing grade Conserves virgin material Saves cost by using in-place “investment” Saves energy by reducing mining and hauls Very sustainable process Advantages of the FDR Process
Benefits of FDR with Cement Increased rigidity spreads loads Eliminates rutting below surface Reduced moisture susceptibility Reduced fatigue cracking in asphalt surfacing Allows for thinner pavement section
Rehabilitation Strategies Attribute Rehabilitation Strategy Reclamation with Cement Structural Overlay Removal and Replacement New pavement structure Fast construction X Minimal traffic disruption XX Minimal material in/out XX Conserves resources XX Maintains existing elevation X Low cost XX
180 12 4,500 300 2,700 0 3,000 500 1 mile of 24-foot wide, 2-lane road, with a 6-inch base Sustainable Element of FDR Process
Laboratory Mix Design Obtain representative samples of roadway material Usually about 100 pounds of material is required Determine the maximum dry density and optimum moisture content at various cement percentages (ASTM D558) Typical designs vary between 2 and 8 percent cement by weight of dry material Prepare samples Cure samples
Strength Determination Unconfined Compressive Strength Testing ASTM D1633 Used by most governing agencies Simple and quick procedure 7-day strengths ranging from 300 to 400 psi are generally recommended Proven strength (support) under extremely heavy traffic conditions Proven performance (durability) in wet-dry and freeze-thaw environments
Please keep in mind that strength and performance are NOT the same thing! The purpose of the mix design procedure is to select the correct amount of stabilizer that most closely balances both strength AND performance for the roadway materials!
Pulverize, Shape, Add Cement, Mix In Place, Compact, and Surface Granular Base Subgrade Existing road Bituminous Surfacing Subgrade Pulverized Pulverization to desired depth Subgrade Pulverized Removal of excess material (if necessary) and shaping Subgrade Stabilized Addition of cement, mixing, reshaping, and compaction Subgrade Stabilized New Surfacing Final surface application FDR Construction Process
Testing Requirements Gradation/UniformityMoisture Density A common density requirement is to be between 96 and 98 percent of the established laboratory standard Proctor density (ASTM D558). A common moisture requirement is to be within 2 percent of the laboratory established optimum moisture content (ASTM D558). A common gradation requirement is for 100 percent to pass a 3-inch sieve, a minimum of 95 percent to pass a 2-inch sieve, and a minimum of 55 percent to pass a No. 4 sieve (ASTM C136).
Traffic and Surfacing Completed FDR base can be opened immediately to low-speed local traffic and to construction equipment Subsequent pavement layers can be placed at any time
PCA Funded Project Study conducted in 2005 Identified candidate project sites in concert with PCA – State (DOT), County, City Agencies, Private Interaction with select officials Visual Pavement Condition Index (PCI) survey Extracted roadway cores for UCS measurements
LTP Study Conclusions Overall, excellent LTP Average PCI of 89 UCS of cores 260 to over 1,000 psi Cement contents 2 to 12 percent with average being 5 percent Most surface distress was in the asphalt layer No major failures attributed to the cement-stabilized base Owners are happy with performance and plan to do more in the future
Concluding Comments Use of in-place materials Very sustainable process Fast operation Constructed under traffic Structurally better than granular base Can apply local traffic almost immediately 30 to 60 percent less expensive than removal and replacement
For more on full-depth reclamation, visit the PCA website at www.cement.org/pavements Questions? For further information please contact: Don A. Clem, PE firstname.lastname@example.org